Effect of Symmetry on the Orientation Distribution. 27 750 Texture, Microstructure & Anisotropy A.D. Rollett. Last revised: 28 th Mar. ‘ 14. Objectives. How to convert Euler angles to an orientation matrix, and back. Review of symmetry for both crystals and materials processing.
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
27750
Texture, Microstructure & Anisotropy
A.D. Rollett
Last revised:28th Mar. ‘14
Sample to Crystal (primed)
^
^
Miller indexnotation oftexture componentspecifies directioncosines of crystaldirections // tosample axes. Form the second axis from the crossproduct of the 3rd and 1st axes.
e’3
e3 // (hkl)
[001]
[010]
^
e’2
^
^
e2 // t
^
e1 // [uvw]
^
e’1
t = hklxuvw
[100]
Obj/notation AxisTransformation Matrix EulerAngles Components
Basic idea: we can construct the complete rotation matrix from two known, easy to determine columns of the matrix. Knowing that we have columns rather than rows is a consequence of the sense of rotation, which is equivalent to the direction in which the axis transformation is carried out.
Obj/notation AxisTransformationMatrixEulerAngles Components
Basic idea: construct the complete orientation matrix from individual, easy to understand rotations that are based on the three different Euler angles. Demonstrate the equivalence between the rotation matrix constructed from these rotations, and the matrix derived from direction cosines. “Rotation” in this context means “transformation of axes”.
Rotation 1 (f1): rotate axes (anticlockwise) about the (sample) 3 [ND] axis;Z1.
Rotation 2 (F): rotate axes (anticlockwise)
about the (rotated) 1 axis [100] axis;X.
Rotation 3 (f2): rotate axes (anticlockwise)
about the (crystal) 3 [001] axis;Z2.
Obj/notation AxisTransformationMatrixEulerAngles Components
Combine the 3 rotations via matrix multiplication; 1st on the right, last on the left:
A=Z2XZ1
Obj/notation AxisTransformationMatrixEulerAngles Components
A = Z2XZ1 =
[uvw]
(hkl)
Obj/notation AxisTransformationMatrixEulerAngles Components
[100]xtaldirection
[010]xtaldirection
[001]xtaldirection
Obj/notation AxisTransformationMatrixEulerAngles Components
TD
ND(hkl)
[uvw]RD
Obj/notation AxisTransformationMatrixEulerAngles Components
[uvw]
(hkl)
[uvw]
(hkl)
≡
Basic idea: the complete orientation matrix that describes an orientation must be numerically the same, coefficient by coefficient, regardless of whether it is constructed from the Euler angles, or from the Miller indices. Therefore we can equate the two matrix descriptions, entry by entry.
Obj/notation AxisTransformationMatrixEulerAngles Components
Compare the matrix formed from the Miller indices with the Euler angle matrix. Extract indices from the 1st and 3rd columns
n, n’ = arbitrary factors to make integers from real numbers
Obj/notation AxisTransformation Matrix EulerAngles Components
Notes: the range of inverse cosine (ACOS) is 0π, which is sufficient for ;from this, sin() can be obtained. The range of inverse tangent is 02π, so numerically one must use the ATAN2(y,x) function) to calculate 1 and 2. Caution: in Excel, one has ATAN2(x,y), which is the reverse order of arguments compared to the usual ATAN2(y,x) in Fortran, C (use ‘double atan2 ( double y, double x ); ‘) etc.!
Also, if the second Euler angle is too close to zero, then the standard formulae fail because sine() approaches zero (see next slide). The second formula deals with this special case, where the 1st and 3rd angles are linearly dependent; distributing the rotation between them is arbitrary.
Corrected a32 in formula for 1 18th Feb. 05; corrected a33=1 case 13th Jan08
A = Z2IZ1 =
Set
I is the Identity matrix
Obj/notation AxisTransformationMatrixEulerAngles Components
The essential points of this lecture are:
Rolling: anvilfire.com
torsion: ejsong.com
{111}
fortharmoury.com
In this case, <100> // F.A.
The essential point about applying a symmetry operation is that, once it has been done, you cannot tell that anything has changed. In other words, the rotated or reflected object is physically indistinguishable from what you started with.
Note the symbols used to denote the different rotational symmetry elements.
[001]
[100]
[010]
[010]
[001]
[100]
Stereographic projectionsof symmetry elements and general poles in thecubic point groupswith HermannMauguinand Schoenfliesdesignations.
Note the presence of four triad symmetry elements in all these groups on <111>.
Cubic metals mostlyfall under .
Groups: mathematical concept, very useful for symmetry
Torsion, shear:Monoclinic, 2.
Rolling, plane straincompression, mmm.
Otherwise,triclinic.
Axisymmetric: C
F
f1
Take a point, e.g. “B”; operate on it with the 3fold rotation axis (blue triad); the set of points related by the triad are B, B’, B’’, with B’’’ being the same point as B. The point is, that as you operate on a point (orientation) with a symmetry operation, in general all the Euler angles change.
[Bunge]
section
in f1 cuts
through
more than
one subspace
Regions I, II and III are
related by the triad crystal symmetry element,
i.e. 120° about <111>, combined with sample symmetry.
[Bunge]
The “S” component,{123}<634>
has angles {59, 37, 63}also {27,58,18},{53,74,34}
and occurs in three
related locations
in Euler space. 10° scattershown about component.
Regions I, II and III are
related by the triad crystal symmetry element,
i.e. 120° about <111>, combined with sample symmetry.
[Randle & Engler, fig. 5.7]
Regions I, II and III are
related by the triad
symmetry element,
i.e. 120° about <111>. 10° scattershown about the S component.
Randle & Engler, fig. 5.7
f1=0°
360°
180°
270°
90°
diad
F
‘mirror’
‘mirror’
= 180°
2fold screw axis changes f2by π
Note: this slide illustrates how the set of 3 diads (+ identity) in sample space operate on a given point. The relationship labeled as ‘mirror’ is really a diad that acts like a 2fold screw axis in Euler space.
Tables for Texture Analysis of Cubic Crystals, Springer Verlag, 1978
3fold axis
360°
180°
270°
90°
f2=0°
F
4fold axis
Other 4fold, 2fold axis:act on f1 also
= 180°
Note: points related by triad (3fold) have different f1 values.
Tables for Texture Analysis of Cubic Crystals, Springer Verlag, 1978
No. of points in the 90x90x90° space
Copper: 2
Brass: 3
S: 3
Goss: 3
Cube: 8
Dillamore: 2
Why this variation?Points that fall on the edge may appear more, or fewer times than the standard count of 3.
Humphreys & Hatherly
f1=0°
360°
180°
270°
90°
diad
F
diad
diad
= 90°
Cube lies on the corners
Copper, Brass, Goss lie on an edge, so that they coincide with a symmetry element
a) Brass b) Copper c) S d) Goss e) Cube f) combined texture
1:{35, 45, 90}, Brass,
2:{55, 90, 45}, Brass
3:{90, 35, 45}, Copper,
4:{39, 66,27}, Copper
5:{59, 37,63}, S,
6:{27, 58,18}, S,
7:{53, 75,34}, S
8:{90, 90, 45}, Goss9: {0, 0, 0}, cube*10:{45, 0, 0}, rotated cube
* Note that the cube exists as a line between (0,0,90) and (90,0,0) because of the linear dependence of the 1st and 3rd angles when the 2nd angle = 0.
Figure courtesy of Jaehyung Cho
Rotation Matrixfrom AxisAngle Pair
Written out as a complete 3x3 matrix:
Matrixrepresentation of the rotation point groups
What is a group? A group is a set of objects that form a closed set: if you combine any two of them together, the result is simply a different member of that same group of objects. Rotations in a given point group form closed sets  try it for yourself!
Note:the 3rd matrix in the 1st column (xdiad) is missing a “” on the 33 element; this is corrected in this slide. Also, in the 2nd from the bottom, last column: the 33 element should be +1, not 1. In some versions of the book, in the last matrix (bottom right corner) the 33 element is incorrectly given as 1; here the +1 is correct.
Kocks, Tomé, Wenk:Ch. 1 Table II
The 4 operators enclosed in orange boxes are also the 222 point group, appropriate to orthorhombic symmetry
g’ = OCg
g’ = OCg
g
Goss: (011)[100]:
=
OC
g
Premultiply by zdiad:
which is (011)[100]
g’
Sample symmetry: right multiply (postmultiply) the matrix.
Euler angles: (52.9, 74.5, 33.7)
Note that all 24 variants are present
Homework exercise: you can make this same plot by using, e.g., Matlab to compute the matrix of each symmetrically equivalent orientation and then converting each new matrix to Euler angles; then use “scatter3” to plot in 3D.
NB: if one writes an orientation as an active rotation (as in continuum mechanics), then the order of application of symmetry operators is reversed: premultiply by sample, and postmultiply by crystal symmetry!
Plots courtesy of VahidTari, 2011
Plots courtesy of VahidTari, 2011
Axis Transformation from AxisAngle Pair
• Since crystal symmetry operators are closely linked to low index directions, it is helpful to convert axisangle descriptions to matrices and vice versa.
• The rotation can be converted to a matrix, g, (passive rotation) by the following expression, whered is the Kronecker delta, is the rotation angle, r is the rotation axis, and e is the permutation tensor.
Compare with active rotation matrix!
Crystal Symmetry Elemente.g. rotation on [001](associated with f2)
[Bunge]
These are simple cases: see detailed charts at the end of this set of slides
Sections at constantvalues of the third angleKocks: Ch. 2 fig. 36

+